2.
A 343/A 343M – 034. Test Specimens 6. Apparatus 4.1 The specimens for this test shall be selected and 6.1 The apparatus shall consist of as many of the followingprepared for testing in accordance with provisions of Practice component parts as are required to perform the desiredA 34/A 34M and as directed in Appendix of this test method. measurement functions: 6.2 Epstein Test Frame:5. Basic Circuit 6.2.1 The test frame shall consist of four solenoids (each 5.1 Fig. 1 shows the essential apparatus and basic circuit having two windings) surrounding the four sides of the squareconnections for this test method. Terminals 1 and 2 are magnetic circuit, and a mutual inductor to compensate for airconnected to a source of adjustable ac voltage of sinusoidal ﬂux within the solenoids. The solenoids shall be wound onwaveform and sufficient power rating to energize the primary nonmagnetic, nonconducting forms of rectangular cross sec-circuit without appreciable voltage drop in the source imped- tion appropriate to the specimen mass to be used. The solenoidsance. All primary circuit switches and all primary wiring shall be mounted so as to be accurately in the same horizontalshould be capable of carrying much higher currents than are plane, and with the center line of solenoids on opposite sides ofnormally encountered to limit primary circuit resistance to the square, 250 6 0.3 mm apart. The compensating mutualvalues that will not cause appreciable distortion of the ﬂux inductor may be located in the center of the space enclosed bywaveform in the specimen when relatively nonsinusoidal the four solenoids if the axis of the inductor is made to becurrents are drawn. The ac source may be an electronic perpendicular to the plane of the solenoid windings.ampliﬁer which has a sine-wave oscillator connected to itsinput and may include the necessary circuitry to maintain a 6.2.2 The inner or potential winding on each solenoid shallsinusoidal ﬂux waveform by using negative feedback of the consist of one fourth of the total number of secondary turnsinduced secondary voltage. In this case, higher primary resis- evenly wound in one layer over a winding length of 191 mm ortance can be tolerated since this system will maintain sinusoi- longer of each solenoid. The potential windings of the fourdal ﬂux at much higher primary resistance. Although the solenoids shall be connected in series so their voltages willcurrent drain in the secondary is quite small, especially when add. The outer or magnetizing winding likewise shall consist ofusing modern high-input impedance instrumentation, the one fourth of the total number of primary turns evenly woundswitches and wiring should be selected to minimize the lead over the winding length of each solenoid. These individualresistance so that the voltage available at the terminals of the solenoid windings, too, shall be connected in series so theirinstruments is imperceptibly lower than the voltage at the magnetic ﬁeld strengths will add. The primary winding maysecondary terminals of the Epstein test frame. comprise up to three layers using two or more wires in parallel. FIG. 1 Basic Circuit for Wattmeter-Ammeter-Voltmeter Method 2
3.
A 343/A 343M – 03 6.2.3 Primary and secondary turns shall be wound in the evaluating the instrument losses. The accuracy of the rmssame direction, with the starting end of each winding being at voltmeter shall be the same as that speciﬁed for the ﬂuxthe same corner junction of one of the four solenoids. This voltmeter. Either digital or analog rms voltmeters are permit-enables the potential between adjacent primary and secondary ted. The normally high-input impedance of digital rms voltme-turns to be a minimum throughout the length of the winding, ters is desirable to minimize loading effects and to reduce thethereby reducing errors as a result of electrostatic phenomena. magnitude of instrument loss compensations. The input resis- 6.2.4 The solenoid windings on the test frame may be any tance of an analog rms voltmeter shall not be less than 5000number of turns suited to the instrumentation, mass of speci- V/V of full-scale indication.men, and test frequency. Windings with a total of 700 turns are 6.5 Wattmeter, W—The full-scale accuracy of the wattmeterrecommended for tests in the frequency range of 25 through must not be poorer than 0.25 % at the frequency of test and at400 Hz. unity power factor. The power factor encountered by a watt- 6.2.5 The mutual inductance of the air-ﬂux compensating meter during a core loss test on a specimen is always less thaninductor shall be adjusted to be the same as that between the unity and, at magnetic ﬂux densities far above the knee of thetest-frame windings to within one turn of the compensator magnetization curve, approaches zero. The wattmeter mustsecondary. Its windings shall be connected in series with the maintain adequate accuracy (1.0 % of reading) even at the mostcorresponding test-frame windings so that the voltage induced severe (lowest) power factor that is presented to it. Variablein the secondary winding of the inductor by the primary current scaling devices may be used to cause the wattmeter to indicatewill completely oppose or cancel the total voltage induced in directly in units of speciﬁc core loss if the combination of basicthe secondary winding of the test frame when no sample is in instrument and scaling devices conforms to the speciﬁcationsplace in the solenoids. Speciﬁcations for the approximate turns stated here.and construction details of the compensating mutual inductor 6.5.1 Electronic Digital Wattmeter—Electronic digital watt-for the standard test frame are given in Table A1.1 of Annex meters have been developed that have proven satisfactory forA1. use under the provisions of this test method. Usage of a 6.3 Flux Voltmeter, Vf—A full-wave true-average, voltme- suitable electronic digital wattmeter is permitted as an alterna-ter, with scale reading in average volts times =2 p/4 so that tive to an electrodynamometer wattmeter in this test method.its indications will be identical with those of a true rms An electronic digital wattmeter oftentimes is preferred in thisvoltmeter on a pure sinusoidal voltage, shall be provided for test method because of its digital readout and its capability forevaluating the peak value of the test magnetic ﬂux density. To direct interfacing with electronic data acquisition systems.produce the estimated precision of test under this test method, 6.5.1.1 The voltage input circuitry of the electronic digitalthe full-scale meter errors shall not exceed 0.25 % (Note 1). wattmeter must have an input impedance sufficiently high thatMeters of 0.5 % of more error may be used at reduced connection of the circuitry, during testing, to the secondaryaccuracy. Either digital or analog ﬂux voltmeters are permitted. winding of the test ﬁxture does not change the terminal voltageThe normally high-input impedance of digital ﬂux voltmeters of the secondary by more than 0.05 %. In addition, the voltageis desirable to minimize loading effects and to reduce the input circuitry must be capable of accepting the maximum peakmagnitude of instrument loss compensations. The input resis- voltage that is induced in the secondary winding during testing.tance of an analog ﬂux voltmeter shall not be less than 1000 6.5.1.2 The current input circuitry of the electronic digitalV/V of full-scale indication. A resistive voltage divider, a wattmeter must have an input impedance of no more than 1 V.standard-ratio transformer, or other variable scaling device Preferably the input impedance should be no more than 0.1 Vmay be used to cause the ﬂux voltmeter to indicate directly in if the ﬂux waveform distortion otherwise tends to be excessive.units of magnetic ﬂux density if the combination of basic In addition, the current input circuitry must be capable ofinstrument and scaling device conforms to the speciﬁcations accepting the maximum rms current and the maximum peakstated above. current drawn by the primary winding of the test ﬁxture when NOTE 1—Inaccuracies in setting the test voltage produce errors ap- core loss tests are being performed. In particular, since theproximately two times as large in the speciﬁc core loss. Voltage scales primary current will be very nonsinusoidal (peaked) if core-should be such that the instrument is not used at less than half scale. Care loss tests are performed on a specimen at magnetic ﬂuxshould also be taken to avoid errors caused by temperature and frequency densities above the knee of the magnetization curve, the cresteffects in the instrument. factor capability of the current input circuitry should be three 6.3.1 If used with a mutual inductor as a peak ammeter at or more.magnetic ﬂux densities well above the knee of the magnetiza- 6.5.2 Electrodynamometer Wattmeter—A reﬂecting-typetion curve, the ﬂux voltmeter must be capable of accurately dynamometer is recommended among this class of instru-measuring the extremely nonsinusoidal (peaked) voltage that is ments, but, if the specimen mass is sufficiently large, ainduced in the secondary winding of the mutual inductor. direct-indicating electrodynamometer wattmeter of the highestAdditionally, if so used, an analog ﬂux voltmeter should have available sensitivity and lowest power-factor capability may bea minimum input resistance of 5000 V/V of full-scale indica- used.tion. 6.5.2.1 The sensitivity of the electrodynamometer wattme- 6.4 RMS Voltmeter, Vrms—A true rms-indicating voltmeter ter must be such that the connection of the potential circuit ofshall be provided for evaluating the form factor of the voltage the wattmeter, during testing, to the secondary winding of theinduced in the secondary winding of the test ﬁxture and for test ﬁxture does not change the terminal voltage of the 3
4.
A 343/A 343M – 03secondary by more than 0.05 %. Also, the resistance of the magnetic ﬂux density without destructive heating or more thanpotential circuit of the wattmeter must be sufficiently high that speciﬁed loss of accuracy due to self-heating. To avoidthe inductive reactance of the potential coil of the wattmeter in intolerable levels of distortion, the value of the resistor shouldcombination with the leakage reactance of the secondary be kept reasonably low. A ﬁxed resistor between 0.1 and 1.0 Vcircuit of the test ﬁxture does not result in appreciable defect is usually appropriate.angle errors in the measurements. Should the impedance of this 6.7.2 Air-Core Mutual Inductor and Flux Voltmeter—Ancombined reactance at the test frequency exceed 1.0 V per air-core mutual inductor and a ﬂux voltmeter may be used to1000 V of resistance in the wattmeter-potential circuit, the measure the peak exciting current. Use of this apparatus ispotential circuit must be compensated for this reactance. based upon the same theoretical considerations that indicate the 6.5.2.2 The impedance of the current coil of the electrody- use of a ﬂux voltmeter on the secondary of the test ﬁxture tonamometer wattmeter should not exceed 1 V. If ﬂux waveform measure the peak magnetic ﬂux density; namely, that when adistortion otherwise tends to be excessive, this impedance ﬂux voltmeter is connected to a test coil, the ﬂux voltmetershould be not more than 0.1 V. The rated current-carrying indications are proportional to the peak value of the ﬂuxcapacity of the current coil must be compatible with the linking the coil. In the case of the air-core mutual inductor, themaximum rms primary current to be encountered during peak value of the ﬂux will be proportional to the peak value ofcore-loss testing. Preferably the current-carrying capacity the current ﬂowing in the primary winding. A mutual inductorshould be at least 10 rms amperes. used for this purpose must have reasonably low primary 6.6 Devices for RMS Current Measurement—A means of impedance so that its insertion will not materially affect themeasuring the rms value of the exciting current must be primary circuit conditions and have sufficiently high mutualprovided if measurements of exciting power or exciting current inductance to provide a satisfactorily high voltage to the ﬂuxare to be made. voltmeter for primary currents corresponding to the desired 6.6.1 RMS Voltmeter and Standard Resistor—A true rms- range in peak magnetic ﬁeld strength. The secondary imped-indicating voltmeter may be used to measure the voltage drop ance of the mutual inductor must be low if any signiﬁcantacross the potential terminals of a standard resistance. The current is drawn by a low-impedance ﬂux voltmeter. Theaccuracy of the rms voltmeter shall be 1.0 % of full scale or addition of the ﬂux voltmeter should not change the mutualless. Either digital or analog meters are permitted. A high- inductor secondary terminal voltage by more than 0.25 %. It isinput-impedance, multirange electronic digital rms voltmeter is important that the mutual inductor be located in the testdesirable for this instrument. The input resistance of an analog equipment in such a position that its windings will not bemeter shall not be less than 5000 V/v. The standard resistor linked by ac leakage ﬂux from other apparatus. Care should beshould be a non-inductive resistor with an accuracy rating of taken to avoid locating it so close to any magnetic material or0.1 % or better. This resistor must be capable of handling the any conducting material that its calibration and linearity mayfull exciting current of the test winding at the maximum test be affected. Directions for construction and calibration of amagnetic ﬂux density without destructive heating or more than mutual inductor for peak-current measurement are given inspeciﬁed loss of accuracy as a result of self-heating. To avoid Annex A1. Even at commercial power frequencies, there canintolerable levels of distortion, the value of the resistor should be appreciable error in the measurement of peak excitingbe kept reasonably low. A ﬁxed resistor between 0.1 and 1.0 V current if winding capacitances and inductances and ﬂuxis usually appropriate. voltmeter errors begin to become important at some of the high harmonics frequencies present because of the extremely non- 6.6.2 RMS Ammeter—A true rms-indicating ammeter may sinusoidal character of the voltage waveform induced in thebe used to measure the exciting current. A nominal accuracy of secondary of the mutual inductor by the nonsinusoidal exciting1.0 % of full scale or better is required for this instrument. The current waveform.instrument must have low internal impedance to avoid contrib- 6.8 Power Supply—A precisely controllable source of sinu-uting to the distortion of the ﬂux waveform. soidal test voltage of low internal impedance and excellent 6.7 Devices for Peak Current Measurement—A means of voltage and frequency stability is mandatory. Voltage stabilitymeasuring the peak value of the exciting current is required if within 0.1 % and frequency accuracy within 0.1 % should bean evaluation of peak permeability is to be made by the maintained. Electronic power sources using negative feedbackpeak-current method. from the secondary winding of the test ﬁxture to reduce ﬂux 6.7.1 Peak-to-Peak Voltmeter and Standard Resistor—The waveform distortion have been found to perform quite satis-peak current measurement may be made with a voltmeter factorily in this test method.whose indications are proportional to the peak-to-peak value ofthe voltage drop across the potential terminals of a standard 7. Procedureresistor connected in series with the primary winding of the test 7.1 Before testing, check the specimen strips for length toﬁxture. This peak-to-peak reading (or peak reading) voltmeter see that they conform to the desired length to within 61⁄32 in.shall have a nominal full-scale accuracy of 1.0 % or better at [0.8 mm] (Note 2). Also check the specimen to see that nothe test frequency and shall be able to accommodate voltages dented, twisted, or distorted strips showing evidence of me-with a crest factor of up to 5. The standard resistor should be chanical abuse have been included and that the strips are ofa non-inductive resistor with an accuracy rating of 0.1 % or uniform width (Note 3). Strips having readily noticeablebetter. This resistor must be capable of handling the full shearing burrs also may be unsuitable for testing. Weigh theexciting current of the test winding at the maximum test specimen on a scale or balance capable of determining the 4
5.
A 343/A 343M – 03mass within an accuracy of 0.1 %. Record specimen weights of that which would be induced in the secondary winding by theless than 1 kg to at least the nearest 0.5 g and within the nearest air ﬂux to be subtracted from that induced by the total ﬂux in1.0 g for specimens heavier than 1 kg. the secondary, the magnetic ﬂux density calculated from the NOTE 2—Inaccuracy in shearing the length of Epstein strips is equiva- voltage indicated by the ﬂux voltmeter is the intrinsic induc-lent to a weighing error of the same percentage. Both weight and specimen tion, Bi = (B −G mHp). In most cases the values of intrinsiclength inaccuracies cause errors in magnetic ﬂux density measurements, induction, Bi, are not sufficiently different from the correspond-which result in even greater core loss errors. ing values of normal induction, B, to require that any distinc- NOTE 3—The width of strips in the specimen should be checked for tion be made. WhereG mHp is not insigniﬁcant compared to Bi,uniformity since nonuniform width will result in nonuniform magnetic as it is at very high magnetic ﬂux densities, determine the valueﬂux density in the specimen, which may have a signiﬁcant but unpredict- of B by adding to Bi either the measured value of GmHp or aable effect upon testing accuracy. nominal value known to be reasonably typical of the class of 7.2 Divide the test specimen strips into four groups contain- material being tested.ing equal numbers of strips, and very closely the same mass, 7.6 Core Loss—When the voltage indicated by the ﬂuxfor testing. Insert the strips (always a multiple of four in voltmeter has been adjusted to the desired value, read thenumber) into the test frame solenoids one at a time, starting wattmeter. Some users, particularly those having wattmeterswith one strip in each of two opposite solenoids and then compensated for their own losses (or burden), will desire toinserting a strip into each of the other two solenoids so that open switch S4 to eliminate the ﬂux voltmeter burden from thethese latter strips completely overlap the former two at the four wattmeter indication. Others will likely choose to have S4 andcorners. This completes one layer of strips constituting a S5 closed when measuring the losses, so that all instrumentscomplete ﬂux path with four overlapped joints. Build up may be read at the same time. In the latter case, the combinedsuccessive layers in this same fashion until the specimen is resistance load of the ﬂux voltmeter, rms voltmeter, andcompletely assembled. With specimens cut half with and half potential circuit of the wattmeter will constitute the totalcross grain, arrange all the parallel or “with-grain” strips in two instrument burden on the wattmeter. Exercise care so that theopposite solenoids and all the cross- or transverse-grain strips combined current drain of the instruments does not cause anin the other two opposite solenoids. appreciably large voltage drop in the secondary circuit resis- 7.3 If the specimen strips are reasonably ﬂat and have a tance of the test frame. In such a case, the true magnetic ﬂuxreasonable area of contact at the corners, a sufficiently low density in the specimen may be appreciably higher than isreluctance is usually obtained without resorting to pressure on apparent from the voltage measured at the secondary terminalsthe joints. When the joints are unavoidably poor, the use oflight pressure on the joints, from the use of nonmagnetic corner of the test frame. In any event, power as a result of any currentweights of about 200 g, is permissible although it may drain in the secondary circuit at the time of reading theintroduce some additional stresses in strain-sensitive materials. wattmeter must be known so it can be subtracted from theWith certain types of magnetic material, or for correct evalu- wattmeter indications to obtain the net watts caused by coreation of properties in certain magnetic ﬂux density ranges, it loss.may be necessary that the specimen be given a heat treatment 7.7 Obtain the speciﬁc core loss of the specimen in watts perto relieve stresses before testing. Follow the recommendations unit mass at a speciﬁed frequency by dividing the net watts byof the manufacturer of the materials in performing this opera- that portion of the mass of the specimen constituting the activetion. magnetic ﬂux path (which is less than the mean geometric path 7.4 Demagnetization—The specimen should be demagne- length) in the specimen. Equations and instructions for com-tized before measurements of any magnetic property are made. puting the active mass of the specimen and the speciﬁc coreWith the required apparatus connected as shown in Fig. 1 and loss are given in 8.2 and 9.2.switches S1, S2, and S4 closed and switches S3 and S5 open, 7.8 Measure the rms value of the secondary voltage byaccomplish this demagnetization by initially applying a voltage having both S4 and S5 closed and the voltage adjusted tofrom the power source to the primary circuit that is sufficient to indicate the correct value of ﬂux volts. On truly sinusoidalmagnetize the specimen to a magnetic ﬂux density above the voltage, both voltmeters will indicate the same voltage show-knee of its magnetization curve (magnetic ﬂux density may be ing that the form factor of the induced voltage is =2 p/ 4.determined from the reading of the ﬂux voltmeter by means of When the voltmeters give different readings, the ratio of thethe equations in 8.1 or 9.1), and then decrease the voltage rms value to that indicated by the ﬂux voltmeter reveals theslowly and smoothly (or in small steps) to a very low magnetic ratio by which the form factor of the induced voltage deviatesﬂux density. After this demagnetization, test promptly for the from the desired value of =2 p/4. Determining the magneticdesired test points. When multiple test points are required, ﬂux density from the readings of a ﬂux voltmeter assures thatperform the tests in order of increasing magnetic ﬂux density the correct value of peak magnetic ﬂux density is achieved invalues. the specimen, and hence that the hysteresis component of the 7.5 Setting Magnetic Flux Density—With switches S3 and core loss is correct even if the waveform is not strictlyS4 closed and switches S1, S2, and S5 open, increase the voltage sinusoidal. But the eddy-current component of the core loss,of the power supply until the ﬂux voltmeter indicates the value being caused by current resulting from a nonsinusoidal voltageof voltage calculated to give the desired test magnetic ﬂux induced in the cross section of the strip, will be in errordensity in accordance with the equations in 8.1 or 9.1. Because depending on the deviation of the induced voltage from thethe action of the air-ﬂux compensator causes a voltage equal to desired sinusoidal wave shape. This error in the eddy-current 5
6.
A 343/A 343M – 03component of loss can be readily corrected by calculations A 5 m/4ld (2)based on the observed form factor and the approximate where:percentage of eddy-current loss for the grade of material being m = total mass of specimen strips, g;tested if the correction is reasonably small. The equations l = length of specimen strips, cm (usually 28 or 30.5 cm);involved in determining this correction are given in 8.3 and and9.3. d = standard assumed density of specimen material (see 7.9 RMS Exciting Current—Measure the rms exciting cur- Practice A 34/A 34M), g/cm3.rent, when required, by having S1 and S4 closed; S2, S3, and S5 8.2 Core Loss—To obtain the speciﬁc core loss of theopen; then with the ammeter on a suitable scale range, adjust specimen in watts per unit mass, it is necessary to subtract allthe voltage to the correct ﬂux voltmeter indication for the secondary circuit power included in the wattmeter indicationdesired test magnetic ﬂux density. When the setting of voltage before dividing by the active mass of the specimen, so that foris correct, open S4 and read the ammeter with no current drain a speciﬁc magnetic ﬂux density and frequency the speciﬁc corein the secondary circuit. If S4 is kept closed to monitor the loss in watts per pound is as follows:magnetic ﬂux density during the current reading, the currentdrain of the ﬂux voltmeter will be included in the ammeter Pc~B; f! 5 453.6 ~Pc 2 E2 2/R!/m1 (3)indication. If exciting current is to be reported in terms ofampere-turns per unit path length, volt-amperes per unit mass, where: Pc = core loss indicated by the wattmeter, W;or permeability from impedance, calculate the values of these E2 = rms value of secondary voltage, V;parameters from the equations of 8.4 and 9.4. R = parallel resistance of wattmeter potential circuit and 7.10 Permeability—When permeability from peak exciting all other connected secondary loads, V; andcurrent is required, determine the peak value of exciting m1 = active mass, g.current using the peak-reading voltmeter and standard resistor. In the 25-cm Epstein frame, it is assumed that 94 cm is theSwitch S1 should be closed to protect the wattmeter from the effective magnetic path with specimen strips 28 cm or longer.possibility of excessive current. Switches S3 and S5 should be For the purpose of computing core loss, the active mass of theopen to minimize secondary loading. With switch S2 open and specimen (less than the total mass) is assumed to be as follows:S5 closed, adjust the voltage to the correct value for the desiredmagnetic ﬂux density or the correct value of peak current for m1 5 l1m/~4l! 5 94m/4l 5 23.5m/l (4)the desired magnetic ﬁeld strength. Equations involved in the where:determination of peak magnetic ﬁeld strength using a peak- m = total specimen mass in pounds;reading voltmeter are given in 8.6 and 9.6. l1 = effective magnetic path length, cm; and 7.11 If the mutual inductor and ﬂux voltmeter are used to l = actual strip length, cm.determine peak current rather than the standard resistor and 8.3 Form Factor Correction—The percent error in formpeak-reading voltmeter, follow the same procedure as in 7.10. factor is given by the following equation:The ﬂux voltmeter used for this purpose must meet the F 5 100~E2 2 Ef!/Ef (5)restrictions of 6.7.2. Equations involved in the determination ofpeak magnetic ﬁeld strength using a mutual inductor and ﬂux assuming (Note 4) that:voltmeter are given in 8.6 and 9.6. observed Pc~B; f! 5 @~corrected Pc~B; f!!/100#h 1 ~corrected Pc~B; f!!Ke/100,8. Calculation (Customary Units) then, the corrected core loss, which shall be computed when 8.1 Calculate the value of the ﬂux voltage Ef at the desired F is greater (Note 5) than 61 %, is:test magnetic ﬂux density in the specimen (when corrected for Corrected Pc~B; f! 5 ~observed Pc~B; f!!100/~h 1 Ke! (6)ﬂux due to H in the material and in the air space encircled bythe test winding through the use of the required air-ﬂux where:compensator) in accordance with the following basic equation observed Pc(B; f) = speciﬁc core loss calculated by thediscussed in X1.2 of this test method: equations in 8.2, h = percentage hysteresis loss at magnetic Ef 5 =2 p BiAN2f1028 (1) ﬂux density B, where: e = percentage eddy-current loss at mag- Bi = maximum intrinsic ﬂux density, G; netic ﬂux density B, and A = effective cross-sectional area of the test specimen, K = (E2/Ef) 2. cm 2; Obviously, h = 100 − e if residual losses are considered N2 = number of turns in secondary winding; and negligible. The values of h and e in the above equation are not f = frequency, Hz. critical when waveform distortion is low. Typical values at 50 8.1.1 In the case of Epstein specimens, where the total or 60 Hz for the common classes of materials, strip thicknesses,number of strips is divided into four equal groups comprising and specimen form are shown in Table 1. Values for materialsthe magnetic circuit, the mass of the specimen in each of the other than those shown may be obtained using core lossfour legs of the magnetic circuit becomes m/4, and the effective separation methods and are a matter of agreement between thecross section, A, in square centimeters, of each leg is: producer and the user. 6
7.
A 343/A 343M – 03 TABLE 1 Eddy-Current Loss (Typical) 8.5.1 For various types of applications, certain types of ac Assumed Eddy-Current Loss, percent (at 50 permeability data are more useful than others. or 60 Hz), for Strip Thicknesses in in. [mm] Material Specimen 8.5.2 One type of ac permeability directly related to the rms 0.007 0.009 0.011 0.012 0.014 0.019 0.025 exciting current (or rms excitation) or ac impedance is char- [0.18] [0.23] [0.27] [0.30] [0.35] [0.47] [0.64] acterized by the symbol µz and is computed as follows (NoteNonoriented half and ... ... ... ... 20 30 40 materialsA half 7):Nonoriented parallel ... ... ... ... 25 35 45 µz 5 Bi/Hz (8) materialsAOriented parallel 35 45 50 50 55 ... ... materialsB where: A Bi = maximum intrinsic ﬂux density, G, and These eddy-current percentages were developed for and are appropriate foruse with nonoriented silicon steels as described in Speciﬁcations A 677/A 677M Hz = ac magnetic ﬁeld strength, Oe (Note 8).and A 683/A 683M where (%Si + 1.7 3 %AI) is in the range 1.40 to 3.70. B These eddy-current percentages were developed for and are appropriate for NOTE 7—For simpliﬁcation and convenience in the calculation of acuse with oriented silicon steels as described in Speciﬁcation A 876/A 876M. permeabilities the value of Bi is used to replace Bm in the permeability equation. This entails no loss of accuracy until the magnetic ﬁeld strength Hp becomes appreciable in magnitude when compared to the value of Bi. If greater accuracy is essential Bm or (Bi + Hp) should be used NOTE 4—In determining the form factor error, it is assumed that the to replace the Bi in these equations.hysteresis component of core loss will be independent of the form factor NOTE 8—Hz is computed from the rms value of the complex excitingif the maximum value of magnetic ﬂux density is at the correct value (as current by assuming a crest factor of =2 . Thus it is based on a sinusoidalit will be if a ﬂux voltmeter is used to establish the value of the magnetic current having a rms value equal to the rms value of the complex current.ﬂux density) but that the eddy-current component of core loss, being afunction of the rms value of the voltage, will be in error for nonsinusoidal 8.5.3 For control work in the production of magneticvoltages. While it is strictly true that frequency or form factor separations materials, it is often desirable to determine an ac permeabilitydo not yield true values for the hysteresis and eddy-current components, value that is more directly comparable to the dc permeabilityyet they do separate the core loss into two components, one which isassumed to vary as the second power of the form factor and the other value for the specimen. This is accomplished by evaluating Hpwhich is assumed to be unaffected by form factor variations. Regardless of from the measured peak value of the exciting current at somethe academic difficulties associated with characterizing these components value of Hp sufficiently above the knee of the magnetizationas hysteresis and eddy-current loss, it is observed that the equation for curve that the magnetizing component of the exciting current iscorrecting core loss for waveform distortion of voltage based on the appreciably greater than the core loss component. Such a testpercentages of ﬁrst-power and second-power of frequency components of point for many commercial materials is an Hp value of 10 Oecore loss does accomplish the desired correction under all practical (796 A/m). Permeability determined in this way is character-conditions if the form factor is accurately determined and the distortionnot excessive. ized by the symbol µp, and is computed as follows (Note 7): NOTE 5—It is recommended that tests made under conditions where the µ p 5 Bi/Hp (9)percent error in form factor, F, is greater than 10 % be considered as likelyto be in error by an excessive amount, and that such conditions be avoided. where Hp is the peak exciting magnetic ﬁeld strength evaluated from measurements of peak current made either with 8.4 Exciting Current—The rms exciting current is often the permeability-inductor or peak-reading-voltmeter methodsnormalized for circuit parameters by converting to the follow- (see 6.7.1 and 6.7.2) and in accordance with the equations ining forms: 8.6. rms exciting force, N1I/l1 5 N1I/94 A2turns/cm ~Note 6! 8.6 Hp from Peak Exciting Current—The peak exciting or ac magnetic ﬁeld strength, Hz 5 0.4p =2N1N/l1 Oe current, Ip in amperes, may be measured using the air-core mutual inductor and ﬂux voltmeter as follows:where: Ip 5 Efm/=2pFLm (10)N1 = number of turns in primary winding;I = rms value of exciting current, A; and where:Hz = ac magnetic ﬁeld strength, Oe. Efm = ﬂux voltage induced in secondary winding of mutual NOTE 6—In previous issues of Test Method A 343, the path length for inductor, V;permeability and exciting current has been taken as 88 cm. In the 1960 and f = frequency, Hz; andsubsequent revisions, the path length has been 94 cm to be consistent with Lm = mutual inductance, H.core-loss determination. The peak exciting current, Ip in amperes, may be computed The speciﬁc exciting power in rms volt-amperes per pound from measurements using a standard resistor and a peak-is: reading voltmeter as follows: Pz~B; f! 5 453.6 E2I/m1 Ip 5 Ep2p/2R1 (11) (7) where:where: Ep-p = peak-to-peak voltage indicated by peak-readingE2 = rms value of secondary voltage, V; voltmeter, V, andI = rms value of exciting current, A; and R1 = resistance of standard resistor, V.m1 = active mass, g. The peak magnetic ﬁeld strength, Hp in oersteds, may be 8.5 Permeability: calculated as follows: 7
8.
A 343/A 343M – 03 Hp 5 0.4pN1Ip/I1 (12) l1 = effective magnetic path length, m.where: 9.3 Form Factor Correction—See 8.3.N1 = number of turns in primary winding; 9.4 Exciting Current—The rms exciting current is oftenIp = peak exciting current, A; and normalized for circuit parameters by converting to the follow-I1 = effective magnetic path length, cm. ing forms: rms exciting force, N1I/l1 5 N1I/0.94 A/m ~Note 9!9. Calculations (SI Units) or 9.1 Calculate the value of the ﬂux voltage Ef at the desired rms ac magnetic ﬁeld strength, Hz 5 =2N1I/l1 A/mtest magnetic ﬂux density in the specimen (when corrected forﬂux as a result of H in the material and in the air space where:encircled by the test winding through the use of the required N1 = number of turns in primary winding;air-ﬂux compensator) in accordance with the following basic I = rms value of exciting current, A; andequation discussed in 1.3 of this test method. Hz = apparent ac magnetic ﬁeld strength, A/m. Ef 5 =2p BiAN2f (13) NOTE 9—In previous issues of Test Method A 343, the path length for permeability and exciting current has been taken as 0.88 m. In the 1960 and subsequent revisions, the path length has been 0.94 m to be consistent Bi = maximum intrinsic ﬂux density, T; with core-loss determination. A = effective cross-sectional area of the test specimen, m2; The speciﬁc exciting power in rms volt-amperes per kilogram is: N2 = number of turns in secondary winding; and Pz~B;f! 5 E2I/m1 (17) f = frequency, Hz. 9.1.1 In the case of Epstein specimens, where the total where:number of strips is divided into four equal groups comprising E2 = rms value of secondary voltage, V;the magnetic circuit, the mass of the specimen in each of the I = rms value of exciting current, A; and m1 = active mass, kg.four legs of the magnetic circuit becomes m/4, and the effectivecross section, A, in square metres, of each leg is: 9.5 Permeability: A 5 m/4ld (14) 9.5.1 For various types of applications, certain types of ac permeability data (in H/m) are more useful than others. where: 9.5.2 One type of ac permeability directly related to the rms m = total mass of specimen strips, kg; exciting current (or rms excitation) or ac impedance is char- l = length of specimen strips, m (usually 0.28 or 0.305 m); acterized by the symbol µz and is computed as follows (Note and 10): d = standard assumed density of specimen material (see µz 5 Bi/Hz Practice A 34/A 34M), kg/m3. (18) 9.2 Core Loss—To obtain the speciﬁc core loss of thespecimen in watts per unit mass, it is necessary to subtract all where:secondary circuit power included in the wattmeter indication Bi = maximum intrinsic ﬂux density, T, andbefore dividing by the active mass of the specimen, so that for Hz = ac magnetic ﬁeld strength, A/m (Note 11).a speciﬁc magnetic ﬂux density and frequency the speciﬁc core NOTE 10—For simpliﬁcation and convenience in the calculation of acloss in watts per kilogram is as follows: permeabilities the value of Bi is used to replace Bm in the permeability Pc~B; f ! 5 ~Pc 2 E2 2/R!/m1 (15) equation. This entails no loss of accuracy until GmHp becomes appreciable in magnitude when compared to the value of Bi. If greater accuracy is where: essential, Bm or (Bi + GmHp) should be used to replace Bi in these equations. The magnetic constant Gm is equal to 4p 3 10 −7H/m. Pc = core loss indicated by the wattmeter, W; NOTE 11—Hz is computed from the rms value of the complex exciting E2 = rms value of secondary voltage, V; current by assuming a crest factor of =2 . Thus it is based on a sinusoidal R = parallel resistance of wattmeter potential circuit and current having a rms value equal to the rms value of the complex current. all other connected secondary loads, V; and m1 = active mass, kg. 9.5.3 For control work in the production of magnetic In the 25-cm Epstein frame it is assumed that 0.94 m is the materials, it is often desirable to determine an ac permeabilityeffective magnetic path with specimen strips 0.28 m or longer. value that is more directly comparable to the dc permeability ofFor the purpose of computing core loss the active mass of the the specimen. This is accomplished by evaluating Hp from thespecimen (less than the total mass) is assumed to be as follows: measured peak value of the exciting current at some value of Hp sufficiently above the knee of the magnetization curve that m1 5 l1m/4l 5 0.94m/4l the magnetizing component of the exciting current is apprecia- 5 0.235m/l bly greater than the core-loss component. Such a test point for (16) many commercial materials is an Hp value of 796 A/m. Permeability determined in this way is characterized by thewhere: symbol µp and is computed as follows (Note 10):m = the total specimen mass, kg; µp 5 Bi/Hpl = the actual strip length, m; and (19) 8
9.
A 343/A 343M – 03 where: TABLE 2 Repeatability and Reproducibility Limits for Speciﬁc Core Loss and Peak Permeability Measurements Hp = peak exciting magnetic ﬁeld strength evaluated from measurements of peak current made either with the NOTE 1—The terms repeatability and reproducibility are used as permeability inductor or peak-reading-voltmeter speciﬁed in Practice E 177. The respective standard deviations among test methods (see 6.7.1 and 6.7.2) and in accordance with results may be obtained by dividing the above limit values by 2.8. the equations in 9.6. ASTM Type 27G051 Material 9.6 Hp from Peak Exciting Current—The peak exciting Speciﬁc Core Loss at 60 Hz Relative Peakcurrent, Ip in amperes, may be measured using the air-core Permeability at and at Maximum Peak Magneticmutual inductor and ﬂux voltmeter as follows: Instrinsic Flux Density, Field Strength, Bi, = Hp, = Ip 5 Efm/=2pfLm (20) 15 kG [1.5 17 kG [1.7 10 Oe [796 A/m] T] T] where: Average Test Value 0.481 W/lb 0.699 W/lb 1840 Efm = ﬂux voltage induced in secondary winding of mutual [1.06 W/kg] [1.54 W/kg] inductor, V; 95 % repeatability 0.6 % 0.7 % 0.12 % f = frequency, Hz; and limitsA 95 % reproducibility 3.4 % 3.1 % 0.62 % Lm = mutual inductance, H. limitsB The peak exciting current, Ip in amperes, may be computed ASTM Type 47S188 Materialfrom measurements using a standard resistor and a peak- Speciﬁc Core Loss at 60 Hz Relative Peakreading voltmeter as follows: and at Maximum Permeability at Ip 5 Ep2p/2R1 (21) Instrinsic Flux Density, Peak Maximum Bi, = Intrinsic Fluxwhere: Density, Bi, = 10 kG [1.0 15 kG [1.5 15 kG [1.5 T]Ep-p = peak-to-peak voltage indicated by peak-reading T] T] voltmeter, V, and Average Test Value 0.698 W/lb 1.67 W/lb 1909R1 = resistance of standard resistor, V. [1.54 W/kg] [3.68 W/kg] The peak magnetic ﬁeld strength, Hp in amperes per meter, 95 % repeatability 0.3 % 0.6 % 1.6 % limitsAmay be calculated as follows: 95 % reproducibility 3.8 % 3.5 % 8.2 % Hp 5 N1Ip/I1 (22) limitsB ASTM Type 64D430 Materialwhere: Speciﬁc Core Loss at 60 Hz Relative PeakN1 = number of turns in primary winding; and at Maximum Permeability atIp = peak exciting current, A; and Instrinsic Flux Density, Peak MaximumI1 = effective magnetic path length, m. Bi, = Intrinsic Flux Density, Bi, = 10 kG [1.0 15 kG [1.5 15 kG [1.5 T]10. Precision and Bias T] T] 10.1 Interlaboratory Test Programs—Two interlaboratory Average Test Value 1.57 W/lb 3.83 W/lb 2291studies have been conducted. In the ﬁrst study, three blended [3.46 W/kg] [8.44 W/kg]Epstein specimens each of ASTM Type 27G051 and ASTM 95 % repeatability 0.2 % 0.3 % 1.1 % limitsAType 47S188 materials were circulated to 14 participating 95 % reproducibility 3.5 % 2.0 % 6.2 %laboratories. in the second study, three blended Epstein speci- limitsBmens of ASTM Type 64D430 material were circulated to 23 A 95 % repeatability limits (within laboratory). Bparticipating laboratories. Practice E 691 was followed for the 95 % reproducibility limits (between laboratories).design of the experiment and the analysis of the data for bothstudies. The details of the studies are given in ASTM Research 10.4 Bias—Since there is no accepted reference material,Report Nos. A06-1000 and A06-1002.6 method, or laboratory suitable for measuring the magnetic 10.2 Test Result—The precision information given below properties determined using this test method, no statement offor core loss or permeability as a percentage of the measured bias is being made.value is for the comparison of two test results, each of whichis a single measurement. 11. Keywords 10.3 Precision—See Table 2. 11.1 alternating-current; ammeter; core loss; customary units; Epstein; exciting power; magnetic; magnetic ﬂux den- 6 Available from ASTM International Headquarters. Request RR: A06-1000 and sity; magnetic material; magnetic test; permeability; powerRR: A06-1002. frequency; voltmeter; wattmeter 9
10.
A 343/A 343M – 03 ANNEXES (Mandatory Information) A1. DETAILS OF CONSTRUCTION FOR EPSTEIN TEST FRAMES AND OTHER COMPONENTSA1.1 Epstein Test Frame the order of 1 or 2 mV or less, the air-ﬂux compensator may be assumed to be adequately compensated. A1.1.1 General principles involved in the construction ofstandard 25-cm Epstein test frames are given in 6.2 of this test A1.2 Crest Ammeter Mutual Inductormethod. Speciﬁc details of wire sizes, turns and dimensional A1.2.1 The permeability mutual inductors, when con-data are given in Table A1.1 of this annex along with the structed in accordance with Table A1.2 of this annex useapproximate electrical characteristics to be expected. tubular winding forms and end disks made from nonconduct- A1.1.2 The standard air-ﬂux compensator, described in a ing, nonmagnetic material and layer wound primary andgeneral way in 6.2.5, uses a tubular (or solid) winding form 2 secondary windings. In this inductor the primary is split, within. [50.8 mm] in diameter by 1 in. [25.4 mm] in length and two one half being wound directly on the winding form, followedend pieces (either square or round) about 4 to 41⁄2 in. [102 to by the full secondary winding, and ﬁnishing with the remaining114 mm] across and 1⁄4 to 1⁄2 in. [6.4 to 12.7 mm] thick. The half of the primary winding. A single thickness of ﬁberwinding form and end pieces may be of any nonconducting, insulating material should be used between each layer of thenonmagnetic material. Screws or bolts used for assembly shall secondary winding to facilitate winding and improve thebe nonmagnetic. The secondary winding is layer wound over frequency characteristics. The two halves of the primary shallthe primary and initially should be comprised of at least 10 % be connected in series. The mutual inductance may be mea-greater number of turns than indicated in Table A1.1 of this sured on a suitable bridge, or the calibration may be made toannex to provide for removal of turns to adjust the secondary acceptable accuracy by passing sinusoidal currents at 60 Hzto the exact number of turns that will completely cancel the through the primary winding and reading the secondary voltagemutual inductance of the solenoid windings. A layer of using the ﬂux voltmeter which is to be calibrated to read Efm ininsulating material a few thousandths of an inch (0.001 terms of crest amperes of exciting current. The mutual inductorin. = 0.0254 mm) thick shall be used between primary and must be so located that no appreciable externally producedsecondary windings. The adjustment of the mutual inductor leakage ﬂux links the secondary winding in the absence of anymay be checked by passing an ac current of 2 to 5 A through primary current. If the secondary current is negligible at thethe primary winding of the test frame with no specimen in the time of measurement the voltmeter will indicate approximatelysolenoids, but with the air-ﬂux compensator connected in 0.12 p ﬂux V/mH of mutual inductance/rms A sinusoidalproper polarity, and observing the open-circuit ac voltage at the primary current (or 0.06 = 2 p ﬂux V/peak A of sinusoidalsecondary terminals with a voltmeter. When this voltage is of primary current/mH). 10
11.
A 343/A 343M – 03 TABLE A1.1 Speciﬁcations for Standard Epstein Frames Having Replaceable Tube Liners NOTE 1—All conductors are enameled copper wire and all turns are close-wound, except that the turns of single layer or incomplete layers shall beuniformly distributed.NominalA specimen weight, kg 2 1 0.5Total turns 700 700 700Approximate secondary voltage at 60 Hz and 15 kG (1.5T) 65 32.5 16.3Dimension of forms: Inner form (liner) inside dimensions, in. 0.750 3 1.25 0.375 3 1.25 0.250 3 1.25 outside dimensions, in. 0.875 3 1.375 0.500 3 1.375 0.375 3 1.375Winding form inside dimensions, in. 0.906 3 1.406 0.563 3 1.406 0.438 3 1.406 outside dimensions, in. 1.031 3 1.531 0.688 3 1.531 0.563 3 1.531Solenoid windings: Primary (top) winding layers 3 3 3 AWG wire size 2 No. 15 (0.057 18 in.) 2 No. 15 (0.057 18 in.) 2 No. 15 (0.057 18 in.) resistance, V 0.57 0.50 0.48 self inductance, mH 1.26 0.99 0.91 Secondary (bottom) winding layers 1 1 1 AWG wire size No. 19 (0.0359 in.) No. 19 (0.0359 in.) No. 19 (0.0359 in.) resistance, V 2.13 1.85 1.75 self inductance, mH 0.85 0.65 0.58Air ﬂux compensator: Dimension of winding form diameter, in. 2.0 2.0 2.0 length, in. 1.0 1.0 1.0 Primary (inner) winding layers 4 4 4 turns 44 44 44 AWG wire size No. 13 (0.072 in.) No. 13 (0.072 in.) No. 13 (0.072 in.) resistance, V 0.06 0.06 0.06 self inductance, mH 0.12 0.12 0.12 Secondary (outer) winding approximate turns 425 315 270 AWG wire size No. 19 (0.0359 in.) No. 19 (0.0359 in.) No. 19 (0.0359 in.) resistance, V 3.5 2.5 2.1 self inductance, mH 15.9 8.6 6.2 Approximate mutual inductance, mH 0.83 0.64 0.57Solenoids and Compensator: Total resistance at primary terminals, V 0.63 0.56 0.54 Total inductance at primary terminals, mH 1.38 1.11 1.03 Total resistance at secondary terminals, V 5.63 4.30 3.82 Total inductance at secondary terminals, mH 16.8 9.3 6.8 A Based on 28-cm-long Epstein strips. 25.4 mm = 1 in. 11
12.
A 343/A 343M – 03 TABLE A1.2 Examples of Standard Crest Ammeter Mutual Inductors For Typical Crest Ammeter UseA BInductor 1 2 3 4Winding form: C Outside diameter, in. [mm] 4 [102] 4 [102] 4 [102] 3 [76] Length, in. [mm] 4 5 / 8 [117] 1 5 / 8 [41] 2 [51] 2 [51] End disk diameter, in. [mm] 8 1 / 4 [210] 7 1 / 2 [191] 9 [229] 9 [229]Primary windings: D AWG wire size E No. 8 sq No. 6 sq No. 9 No. 8 Layers 8 4 6 12 Turns F 240 32 96 156Secondary Windings: B AWG wire size E No. 28 No. 28 No. 22 No. 16 Layers 32 32 41 17 Turns 8640 3200 1540 546Electrical characteristics: Primary self inductance, mH 5.01 0.14 1.7 2.35 Primary resistance, V 0.25 0.023 0.14 0.10 Secondary self inductance, mH 7350 1650 800 50.98 Secondary resistance, V 860 296 65 3.65 Mutual inductance, F mH 181.2 12.9 35.1 7.066 A To maintain accuracy, the ﬂux voltmeter should not draw any appreciable current that can change the mutual inductor secondary“ Terminal” voltage (see 6.7.1). B In Inductors 1, 2, and 3, generally the primaries are divided into two sections by the secondary, that is, one-half the primary turns are placed on the form ﬁrst; thecomplete secondary winding second, and the remaining one-half of the primary turns placed on top of the secondary. The top and bottom primary windings shall beconnected in series. C The tubular winding form and the end disks shall be made of nonmagnetic, nonconducting material. Other parts of the winding form shall be nonmagnetic. D An insulating layer of paper should be placed between windings. E All conductors are at least enamel insulated. F It may be desirable to make the crest ammeter direct reading in peak oersteds or peak A/m. This inductor may be tapped for this purpose if desired. A2. RECOMMENDED STANDARD TEST VALUESA2.1 Standard Test Values A2.1.1.2 Tests for ac permeability from peak exciting cur- A2.1.1 For tests at 50 or 60 Hz on ﬂat-rolled materials in rent (if required) at a magnetic ﬂux density of 15 kG [1.5 T] orstandard thicknesses, the following test points are recom- at a magnetic ﬁeld strength of 10 Oe [796 A/m].mended: A2.1.1.1 Test for core loss (and rms exciting current ifrequired) at magnetic ﬂux densities of 10, 15, or 17 kG [1.0,1.5, or 1.7 T], and A3. PREPARATION OF EPSTEIN TEST SPECIMENSA3.1 Test Specimens strip length (2-, 1-, or 0.5-kg total mass in 28-cm [280-mm] A3.1.1 When magnetic properties of the basic magnetic strip length) as determined by the instrumentation and testmaterial are desired (with effects of specimen shape, joints in frame dimensions (Note A3.1). In no case shall the specimenthe magnetic circuit, and characteristics of the test windings consist of less than 12 strips. Specimens weighing less than 15reduced to negligible proportions), the test specimen shall, g/cm [1.5 g/mm] of strip length shall consist of at least 20whenever possible, consist of strips (commonly called Epstein strips. In all cases, the specimen is subject to the requirementstrips) arranged in an Epstein frame so as to constitute a square that the strips be taken so as to adequately represent the areasmagnetic circuit with the strips completely overlapped (double being sampled, and that the total number of test strips be alapped) at the corners. Flat-rolled magnetic materials supplied multiple of four. Table A3.1 gives the number of stripsas sheets or coils preferably shall be tested in this specimen frequently used to meet this requirement for various stripform whenever dimensions permit. thicknesses. A3.1.2 The Epstein test specimens shall consist of strips cutfrom sheets or coils in accordance with Practice A 34/A 34M. NOTE A3.1—The dimensions of the winding form of the test frameThe strips shall be 3.00 cm [1.181 in. or 30 mm] in width and should be suitable for accommodating the desired specimen mass withoutnot less than 28.0 cm [11.02 in. or 280 mm] in length. If, for excessive unﬁlled space within the test windings. Standard test frames (see 6.2) are designed with dimensions accommodating nominal specimenease of assembly and disassembly of the specimen in the test weights of 2, 1, or 0.5 kg. Increased sensitivity of instruments will beframe, it is desired to use strips slightly longer than 28.0 cm necessary for adequate performance on specimens of smaller than nominal[280 mm], a length of 30.5 cm [12.01 in. or 305 mm] is weight. Specimens weighing less than about one half the nominal mass forrecommended. the test frame dimensions should not be used unless the instrumentation of A3.1.3 The nominal mass of an Epstein test specimen shall the test equipment has been speciﬁcally designed for operation under suchbe approximately 71.5, 36, or 18 g/cm [7.15, 3.6, 1.8 g/mm] of conditions. 12
13.
A 343/A 343M – 03 FIG. A3.1 Suggested Distribution of Strips to Be Cut from Sheets for Magnetic Tests TABLE A3.1 Suggested Number of Test Strips material has been rolled and half transverse or across the Number of 280-mm Long Strips for Test Specimens of direction of rolling, it is recommended that sufficient strips be Nominal MassStrip Thickness, in. [mm] cut in accordance with the arrangement indicated in Fig. A3.1 500 g 1000 g 2000 g (a) or (b). Where the material has been produced as continuous 0.0310 [0.79] 12 20 40 cold-reduced coils, sufficient length should be discarded from 0.0280 [0.71] 12 24 44 0.0250 [0.64] 12 24 48 the end of the coil to insure uniform properties in the test strips. 0.0220 [0.56] 16 28 56 A3.1.5 If the test specimen comprises only parallel or 0.0185 [0.47] 16 32 64 0.0170 [0.43] 20 36 72 “with-grain” strips, it is recommended that sufficient strips be 0.0155 [0.39] 20 40 80 cut in accordance with Fig. A3.1 (c). 0.0140 [0.36] 24 44 88 0.0125 [0.32] 24 48 96 A3.1.6 When less than the total number of strips obtained 0.0110 [0.28] 28 56 112 from the sampled area are needed for the test specimen, the 0.0090 [0.23] 36 68 136 0.0070 [0.18] 44 88 176 excess strips should be discarded equally from all locations in the sampled areas. For instance, if approximately one fourth of the total strips obtained is excess, every fourth strip should be A3.1.4 If the specimen is to comprise strips with half the discarded.total number cut parallel or with the direction in which the APPENDIXES (Nonmandatory Information) X1. BASIC PRINCIPLES AND DEVELOPMENT OF EPSTEIN TEST EQUATIONSX1.1 Basic Principles X1.1.5 Alternating-current normal induction, B, shall be X1.1.1 The basic features involved in these alternating- determined (in accordance with X1.2 or X1.3) from measure-current methods, which should be strictly adhered to by the ments made with a voltmeter responsive to the full-waveuser unless otherwise stated in the individual test methods, are average value of the voltage (rectifying-type voltmeter), com-as follows: monly called a ﬂux voltmeter,7 connected to an essentially unloaded secondary winding enclosing the specimen. The ﬂux X1.1.2 The test specimen shall be of uniform cross section voltmeter shall conform to the speciﬁcations given in theperpendicular to the direction of the ﬂux path and should have individual test methods.uniform properties in any given direction. X1.1.6 The value of the effective test specimen cross- X1.1.3 The ﬂux waveform, as judged by the form factor of sectional area shall be determined from mass, length, andthe voltage wave induced in an unloaded secondary winding, density of the test specimen wherever feasible (Practice A 34/shall be sinusoidal within limits described in the individual test A 34M). Equations for calculating this area are given in themethods. To accomplish this, the power source must generate individual test methods.a closely sinusoidal waveform, and the primary circuit imped-ance (including the power source) shall be kept as low as 7possible. See, Camilli, G., “A Flux Voltmeter for Magnetic Tests,” Journal, American Institute of Electrical Engineers., JAIEE, Vol 45, October 1926, p. 721; also Smith, X1.1.4 Voltage and frequency shall be very closely con- B. M., and Concordia, C., “Measuring Core Loss at High Densities,” Electricaltrolled within limits given in the individual test methods. Engineering, ELENA, Vol 51, No. 1, January 1932. 13
Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.
Be the first to comment